Characterization of Polymers by Matrix
Macromolecules 1995,28, 4562-4569
Characterization of Polymers by Matrix-Assisted Laser
Desorption Ionization-Time of Flight Mass Spectrometry. End
Group Determination and Molecular Weight Estimates in
Dipartimento di Scienze Chimiche, Universita di Catania, Viale A. Doria,
6-95125 Catania, Italy
Maurizio S. Montaudo, Concetto Puglisi, and Filippo Samperi
Istituto per la Chimica e la Tecnologia dei Materiali Polimerici, Consiglio Nazionale delle
Ricerche, Viale A. Doria, 6-95125 Catania, Italy
Received August 29, 1994; Revised Manuscript Received January 20, [email protected]
ABSTRACT: Matrix-assisted laser desorption ionization-time of flight mass spectrometry (MALDITOF MS) allows mass measurements of large molecules such as those present in synthetic and natural
macromolecules. We have used a self-calibrating method for the MALDI-TOF spectra of polymers,
enabling us to obtain accurate mass values. Poly(ethy1ene glycol) (PEG) samples having two different
(ii) cationic PEG,
kinds of end groups were used in our work: (i) anionic PEG, H-(CHz-CHz-O),-H;
The MALDI-TOF spectra recorded in reflected mode allowed unambiguous
identification of the end groups present in these PEG samples. Five anionic PEG samples with very
narrow molecular weight distributions (MWD) were studied. The MALDI-TOF spectra of PEGS were
recorded in both linear and reflected modes. Due to the high sensitivity and the highly linear response
of HIMAS (a microchannel detector equipped with a photomultiplier), measurements of MALDI-TOF
spectra were used in our work to estimate the MW and MWD of the PEG samples. Our results show
that the molecular weight estimates provided by MALDI-TOF measurements agree with the values
obtained by conventional techniques such as GPC, osmometry, and viscometry.
Matrix-assisted laser desorption ionization-time of
flight mass spectrometry (MALDI-TOF MS) is a recently introduced1,2soft ionization technique that allows
desorption and ionization of very large molecules even
if in complex mixtures, such as the wide molecular
weight distributions (MWD) present in synthetic and
The great promise of MALDI-TOF is to perform the
direct identification of mass-resolved polymer chains,
including intact oligomers within a MWD, measurement
of MW and of MWD, and the simultaneous determination of end groups in polymer samples.
This perspective has stirred much expectation among
polymer scientists. The MALDI-TOF technique was
originally developed for proteins,lP2and its extension to
the characterization of synthetic polymers is still
The task of obtaining accurate mass values in MALDI-TOF spectra of synthetic polymeric materials is of
utmost importance, since it would make possible the
direct determination of the composition of the species
contained in each polymer sample and also of different
end groups present in the oligomer series. End group
identification and determination of the actual composition (down to species present to minor amounts) of a
polymer sample are crucial in polymer analysis, and
their importance cannot be overemphasized.
Problems may also be encountered in determining
molecular weights of polymers from their MALDI-TOF
spectra. The intensity of mass peaks in mixtures is
proportional to the molar amount of each species, and
therefore mass spectra of polymers yield the number
Abstract published in Advance ACS Abstracts, May 1, 1995.
average MW (although other averages may be calculated using appropriate algorithms), whereas GPC
yields weight averages (although other averages may
be calculated also here). This has to be taken into
account when results are compared from the two
techniques on polydisperse samples. Furthermore, in
order to give a correct MW estimate, the MALDI-TOF
detector must show a constant response to ions over a
wide range of mass numbers.
In the following, we report a MALDI-TOF study of
PEG samples having very narrow MWD and address
some of the points listed above.
Anionic PEG Samples. PEG samples were purchased by
Polymer Laboratories. They were prepared by anionic polymerization of ethylene oxide initiated with potassium alcoholate
in the presence of excess alcohol. Table 1 gives the average
molecular weights, obtained by different methods for the five
PEG samples, as given by the sample supplier.
Cationic PEG Sample. The PEG2000 sample was obtained from Fluka. It was synthesized by reacting ethylene
oxide with an excess of water in the presence of acid catalyst
MALDI Sample Preparation. 2-((4-Hydroxyphenyl)azo)benzoic acid (HABA) was used as a matrix, and tetrahydrofuran, as a solvent. In the case of PEG2000, the solvent was
ethanol and the matrix was dihydroxybenzoicacid. Probe tips
were loaded with 100 pmol of polymer sample and 300 nmol
MALDI-TOF Mass Spectra. A Bruker REFLEX mass
spectrometer (Bruker Franzen Analytik, Bremen, Germany)
was used to obtain the matrix-assisted laser desorption
ionization-time of flight mass spectra. The spectrometer was
equipped with a nitrogen laser (337 nm, 5 ns) and a flash ADC
(time base 8 ns). The length of the drift tube is about 1.2m.
The detection in the linear mode was achieved by means of a
HIMAS detector. It has a venetian-blind steel dynode which
0 1995 American Chemical Society
Macromolecules, Vol. 28,No. 13, 1995
Polymer Characterization by MALDI-TOF 4563
Table 1. Molecular Weight Averages and Molecular Weight Distributions for PEG Samples
a Vapor pressure osmometry, as measured from the sample supplier. b Membrane osmometry, as measured from the sample supplier.
Light scattering, as measured from the sample supplier. Intrinsic viscosity, as measured from the sample supplier. e Estimated from
GPC by the sample supplier. f Most probable mass estimated from the MALDI-TOF linear spectrum. g Most probable mass estimated
from the MALDI-TOF reflection spectrum. Computed from the MALDI-TOF linear spectrum by equation M , = LNGMJNL.Computed
from the MALDI-TOF linear spectrum by equation M , = ZN5(ML)2/NJtfL.
1 Calculated from the values in the last two columns.
performs the ion-to-electronconversion. Ehctrons pass through
a 6000 V potential difference and hit first a single-plate
microchannel detector and then a cesium iodide scintillator
which surmounts the entrance window of a photomultiplier.
The conversion dynode enables the detection of high-massions.
The scintillator avoids the detector saturation by providing a
very wide dynamic range. The HIMAS detector has low
temporal resolution. This is probably due to the production
of secondary ions by the conversion dynode. The detection in
the reflected mode was achieved by the standard double-plate
microchannel detector. The accelerating voltage was 30 kV.
The laser irradiance was slightly above threshold (ca. lo6
W/cm2). Ions below m l z 350 were removed with pulsed
deflection, and 100 transients were summed. The resolution
at 5000 Da was 300 in the linear mode and 500 in the reflected
Results and Discussion
The determination of accurate masses in the MALDI
spectra of synthetic polymers that may in fact be
mixtures and may possess different end groups can
sometimes be a difficult task.14
The TOF spectrum is initially obtained as a temporal
spectrum, which reports the number of ions arriving at
each time. The mass spectrum is then usually calibrated by recording the spectrum of a compound of
known mass and computing the set (Q) of calibration
constants. The set Q is then used to calibrate the
spectra of the unknown sample. The accuracy in mass
determination by this procedure is claimed4J5 to be 0.1%
(i.e. 10 mass units a t 10 000). Such a low level of
accuracy is related to the fact that each mass spectrum
has its own set Q, which varies when passing from one
spectrum to another.
For end group determinations by MALDI-TOF spectrometry, the accuracy in mass determination by the
external calibration procedure is not enough and one
needs a n accuracy of about 0.02%. We have used a selfcalibrating method for the MALDI-TOF spectra of
polydisperse polymers, which enables us to obtain an
accuracy of about 0.02% for masses up to 1000020 O0O,l2 as discussed below.
The time (ti) needed for a n ion of mass pcalc(i)to fly
through the tube and the mass of the ion itself are
= a(ti+ 10
where a and B are calibration constants, whose values
must be found through a process involving tentative
assignments of the peaks in the spectra and by a linear
regression p r ~ c e d u r e . ~
In the case of polymeric materials, however, one can
take advantage of a unique property of the latter.
Considering that the mass of a homopolymer results
from the sum of identical units, eq 1 can be coupled with
the condition that the mass of each oligomer results
from the sum of a multiple of 0,the mass of the polymer
repeat unit, and 8, the mass of the first peak considered
in the process of enumerating mass spectral peaks.
Then, within the same mass series, the distance
between two adjacent ions is a multiple of u,and the
exact mass of the ion pmulti(i), is
= (i - l ) u
The calibration procedure consists in varying a and /3
until pcalc equals pmulti. This is done by minimizing the
sum of squares:
where the summation goes from 1to n ( n is the number
of peaks in the mass series). The computation of the
point of minimum, P, is cumbersome. In order to
circumvent this obstacle, it is useful to introduce a
function SS2, similar to SS1.
It is reasonable to assume that, if SS1 has a minimum
at point P, then also SS2 takes its minimum value at
point P. A computer program, called CALTOF,16 was
developed in order to find the minimum of SS2 in eq 4.
I t accepts as input u (the mass of the polymer repeat
unit) and the time of flight (ti) corresponding to peaks
in the MALDI-TOF mass spectrum. I t gives as output
and pmulti(i),the calibration constants
the vectors pcalc(i)
a and ,!I,
and the plot of SS2 as a function of 8.
In Figure 1 are reported four minimization curves,
obtained by the calibration procedure described above.
As discussed above, the procedure takes advantage of
the finding that SS2 takes its minimum a t 8, the mass
of the first oligomer appearing in the MALDI-TOF
spectrum. Since 0 is also known (being the repeat unit
of the polymer), eqs 1 and 2 can be solved and the
masses can be calculated. The mass accuracy obtained
was about 0.02% at resolution 500, based on the
comparison between the mass values found and those
expected from the polymer formula (i.e., repeat units
plus end groups plus cation). The MALDI spectra of
the PEG samples were calibrated by following this
procedure and are discussed below.
Parts a and b of Figure 2 report the MALDI-TOF
mass spectra of PEG4100, measured in linear and
reflected mode, respectively. The reflected spectrum
(Figure 2b) shows a higher resolution (mlAm = 500)
compared to that in linear mode (Figure 2a), so that two
mass series can be discerned (see inset).
The anionic PEG samples investigated here (Table 1)
were obtained by ring-opening polymerization of ethylene oxide initiated with potassium alcoholate in the
presence of excess alcohol, acting as transfer agent and
MW regulator. Assuming that the reactivities of all the
OH functions in the transfer process are the same,
Macromolecules, Vol. 28, No. 13, 1995
4564 Montaudo et al.
alfa = 844412
beta = 4
alfa = 844081
beta = 22
alfa = 843992
beta = 16
alfa = 844380
Figure 1. Plots of the function SS2 in eq 4 as a function of q for samples PEG4100, PEG7100, PEG8650, and PEG12600.
independent of the chain length, the number average
degree of polymerization of the poly(ethy1ene oxide)
formed is given by the molar ratio of monomer and
alcohol involved. The reaction scheme can be written
C H ~ - C H Z - O - ( C H ~ - C H ~ - O )-CHz-CHz-OH
The latter formula can be rewritten as H-(CHz-CHz0),+1-H, from which the MW of each PEG oligomer can
be calculated: (44.03n 2). If the PEG ions appear as
Na' or K+ adducts, then their mass shall be given by
( 4 4 . 0 3 ~ ~2 23) or ( 4 4 . 0 3 ~ ~2 39), respectively.
The MALDI-TOF spectrum in Figure 2b was calibrated
with our procedure. The CALTOF computer program
gave as output a = 844 412, ,L? = 4.0 (eq 1). Therefore,
the most intense mass series appearing in Figure 2b is
associated with ions of the type: (44.03n 2 23), and
the second with ions of the type (44.03n 2 39). PEG
ions appear therefore as Na+ and Kf adducts in the
the peaks appearing in the MALDITOF spectrum of a PEG sample were measured to have
substantial mass differences from those reported above,
well beyond the experimental uncertainty. For instance, the 27mer was assigned mass number 1229.7
Da (instead of 1213.8 Da), and the 37mer was assigned
mass number 1670.0 Da (instead of 1654.1 Da). These
mass values appear to correspond to a formula (44.03n
18 231, where the PEG oligomers are terminated
by hydroxy groups, and we thought therefore that they
originated from a PEG sample prepared from ethylene
oxide and water in the presence of a n acidic catalyst. A
sample (PEG2000), obtained by the latter synthetic
method, was then analyzed (Figure 2C), and it was
found to have the mass values expected for the formula
( 4 4 . 0 3 ~ ~18 23).
This experiment shows that MALDI analysis can
distinguish two PEG polymers terminated by different
In Figure 3a,b are reported the MALDI-TOF mass
spectra of PEG 7100, measured in the linear and
reflected modes, respectively. As in the previous case,
the reflected spectrum shows a higher resolution compared to that in linear mode, so that the two mass series
corresponding to Na+ and K+ adducts of PEGS can be
distinguished. The same result was obtained in the case
of PEG8650 (omitted for brevity) and of PEG12600. In
the latter case, shown in Figure 4a,b, the peaks in the
reflected spectrum are broader than for PEG7100. As
a consequence, the peaks due to K+ adducts are no more
resolved from the peaks due to Na+ adducts. The peak
broadening at high masses is a well-known feature of
In Figure 5a,b are reported the MALDI-TOF mass
spectra of PEG23600, measured in the linear and
reflected modes, respectively. I t can be seen that the
spectrum is not mass resolved and therefore it is
impossible to distinguish the peak due to one oligomer
from that of another. In fact, in this mass range, peaks
are quite broad (the width of peaks in the reflected
spectrum were estimated to be 50-55 Da), so that the
signal due to a given oligomer is not resolved from the
signals of its nearest neighbors (the spacing between
neighboring peaks is 44 Da). The noise level of the
reflected spectrum in Figure 5b appears to be acceptable, but this result was obtained only after digital
filtering (smoothing) of the raw data. In fact, the
original S/N ratio was 5 times worse. As a matter of
fact, ions strike against and reflected detector, but they
produce a very small signal. This is due to the characteristics of the detector, and it has been shown that
the sensitivity of this detector varies with the velocity
Macromolecules, Vol. 28,No.13, 1995
Polymer Characterization by MALDI-TOF 4565
Figure 2. MALDI-TOF spectrum for sample PEG4100 in the linear mode (a), for sample PEG4100 in the reflected mode (b),
and for sample PEG2000 in the reflected mode (e).
Macromolecules, VoZ. 28, No. 13, 1995
4566 Montaudo et al.
I ~ ' " ~ ' ~ ' ' " ' ~ ~ " ' ' I " ' ' I ' ~ ' ' I ' ' ~ ~ ~
111 I I
12000 m l r
Figure 3. MALDI-TOF spectrum for sample PEG7100 in the linear (a) and the reflected mode (b).
Polymer Characterization by MALDI-TOF 4567
Macromolecules, Vol. 28, No. 13, 1995
Figure 4. MALDI-TOF spectrum for sample PEG12600 in the linear (a) and the reflected mode (b)
Macromolecules, Vol. 28, No. 13, 1995
4568 Montaudo et al.
Figure 5. MALDI-TOF spectrum for sample PEG23600 in the linear (a) and the reflected mode (b).
Macromolecules, Vol. 28, No. 13, 1995
of the incoming ions.18 The difficulties associated with
the detection of large masses can be circumvented by
using a detector in which the conversion from ions into
electrons is performed outside the microchannel plate. l9
The linear detector possesses this characteristic and is
therefore well-suited for the detection of large masses.
The MALDI spectra of PEG23600 in Figure 5a,b clearly
slow also the appearance of a PEG dimer at m/z 47 000.
Furthermore, two peaks appear in the spectra: one, less
intense, a t mlz 18 500 and another at mlz 23 600. This
PEG sample appears to have a bimodal distribution of
M W , a fact not detected by GPC (Table 1). In the linear
mode, the ratio between the intensities of the peak at
23 600 and 18 500 Da is about 5 . In the reflected mode,
this ratio is instead about 2. This is due to the fact that
the reflected detector response falls a t high masses. The
signal-to-noise ( S N ) ratio in the linear spectrvm is good.
A comparison between the mass spectra in Figures 2-5
shows that the SIN ratio of the reflected spectra worsens
appreciably at high masses, wheres the S/Nratio of the
linear spectra remains nearly constant with varying
Table 1gives the average molecular weights for the
five PEG samples investigated by MALDI-TOF together with the values given by the supplier, as obtained
by different methods.
Due to the high sensitivity and highly linear response
of the HIMAS detector (see Experimental Section),
measurements of MALDI-TOF spectra in the linear
mode were used in our work to estimate the MW and
MWD of the PEG samples. The reflected detector in
our instrument design has different characteristics from
the HIMAS (see Experimental Section), and it is less
useful for MW measurements since its sensitivity falls
beyond about 30-40 kDa (but its resolution increases).
We have recorded the MALDI-TOF spectra also in
the reflected mode in order to take advantage of the
higher resolution of these spectra for end group identification purposes. Nevertheless, from Table 1 it can
be seen that the MALDI-TOF spectra provide wellcomparable estimates for the most probable (M,)
values, as measured independently from the linear and
reflected spectra. This fact is due to the relatively low
MW values of the PEG samples investigated.
Data in Table 1also show that the molecular weight
estimates provided by MALDI-TOF measurements
agree with the values obtained by conventional techniques. M, values derived from MALDI-TOF spectra
in the linear mode agree well with the Mn values
obtained from osmometry and viscosity measurements
(Table 1).Also the Mpvalues estimated from GPC come
close t o the Mp values observed in the MALDI-TOF
spectra. It ought t o be remarked that Mn values are
all lower than Mp. The reason is that the MWD is not
symmetrical with respect to its maximum. In fact,
MWD has a “tail” at low masses. In the case of sample
PEG23600, the value Mp = 23 710 Da, estimated from
the MALDI-TOF spectrum in the linear mode (Figure
5a), differs significantly from the calculated value of M ,
= 21 450 Da because the latter was obtained by taking
into account the bimodal distribution shown by the
spectrum in Figure 5a.
Comparing the GPC and MALDI-TOF Mw/Mnratios
in Table 1, it appears that the MALDI-TOF spectra
Polymer Characterization by MALDI-TOF 4569
yield an appreciably narrower dispersity index with
respect to GPC. The disagreement may not appear
serious for these samples, prepared by anionic polymerization and therefore possessing quasi-Poisson distributions. However, for samples showing Flory distributions, or even wider, MALDI-TOF spectra may yield
Summarizing our results of the characteristics of
PEGS by MALDI-TOF mass spectra, we have used a
calibration procedure especially useful for end group
identification and have performed a comparison of MW
and MWD estimates by MALDI-TOF and conventional
techniques (including GPC). The PEG samples investigated here possess a very narrow MWD; we shall
report later on the characterization by MALDI-TOF of
polymeric samples of wider MWD.20
Acknowledgment. Partial financial support from
the Italian Ministry for University and for Scientific and
Technological Research (MURST) and from the National
Council of Research (CNR, Rome) is gratefully acknowledged.
References and Notes
(1) Karas, M.; Hillenkamp, F. Anal. Chem. 1988, 60, 2299.
(2) Hillenkamp, F.; Karas, M.; Beavis, R. C.; Chait, B. T. Anal.
Chem. 1991,63, 1193A.
(3) Bahr, U.; Deppe, A.; Karas, M.; Hillenkamp, F.; Giessman,
U. Anal. Chem. 1992, 64, 2866.
(4) Cotter, R. A. Anal. Chem. 1992, 64, 1027A.
(5) Bruker. User Software Manual, Reflex MALDI-TOF Bruker: Bremen, Germany, 1993.
(6) Danis, P. 0.;Karr, D. E.; Mayer, F.; Holle, A.; Watson, C. H.
Org. Mass Spectrom. 1992, 27, 843. Danis, P. 0.;Karr, D.
E. Org. Mass Spectrom. 1993,28, 923.
(7) Danis, P. 0.;Karr, D. E.; Westmoreland, D.; Piton, M. C.;
Christie, D. I.; Clay, P. A.; Kable, S. H.; Gilbert, R. G.
Macromolecules 1993,26, 6684.
(8) Burger, H. M.; Muller, H. M.; Seebach, D.; Bornsen, K. 0.;
Schar, M.; Widmer, H. M. Macromolecules 1993, 26, 4783.
(9) Eggert, M.; Freitag, R. J . Polym. Sci., Part A: Polym. Chem.
(10) Visy, C.; Lukkari, J.; Kankare, J. Macromolecules 1994,27,
(11) Abate, R.; Ballistreri, A.; Montaudo, G.; Garozzo, D.; Impallomeni, G.; Critchley, G.; Tanaka, K. Rapid Commun. Mass
Spectrom. 1993, 7, 1033. Garozzo, D.; Spina, E.; Sturiale,
L.; Montaudo, G . Rapid Commun. Mass Spectrom. 1994, 8 ,
(12) Montaudo, G.; Montaudo, M. S.;Puglisi, C.; Samperi, F. Anal.
Chem. 1994,66,4366;Rapid Commun. Mass Spectrom. 1994,
(13) Ehring, H.; Karas, M.; Hillenkamp, F. Org. Mass Spectrom.
1992.27.472. Beavis. R. C.: Chaudharv. T.: Chait. B. T. O w .
Mass’ Spectrom. 1992; 27, 156.
(14) However, this is not strictlv true in the case of MALDI-FT
mass spectra. See, e.g.: Castox-o, J. A.; Wilkins, C. L. Anal.
. . Zaia. J.: Annan. R. S.: Biemann. K. Ranid Commun. Mass
Spectrom. 1992; 6, 32.’
(16) CALTOF DaDer listinn available on reauest.
(17) Hillenkamp,-F. Procegdings of the fifth ;nternational conference on biological mass spectrometry held in Kyoto 1992;
Springer: Berlin, 1992; p 22.
(18) Gross, M. L., Ed.; Mass spectrometv in the biological sciences:
a tutorial; Kluwer: New York, 1992; p 133.
(19) Spengler, B.; Kirsh, D.; Kaufmann, R.; Karas, M.; Hillenkamp, F.; Geissmann, U. Rapid Commun. Mass Spectrom.
1992, 6, 32.
(20) Montaudo, G.; Montaudo, M. S.; Puglisi, C.; Samperi, F.
Rapid Commun. Mass Spectrom. 1995, 9, 453.